1 CHAPTER 2 Fundamentals of the Heat Treating of Steel BEFORE CONSIDERATION can be given to the heat treatment of steel or other iron-base alloys, it is helpful to explain what steel is. The common dictionary definition is a hard, tough metal composed of iron, alloyed with various small percentage of carbon and often variously with other metals such as nickel, chromium, manganese, etc. Although this definition is not untrue, it is hardly adequate. In the glossary of this book (see Appendix A, Glossary of Heat Treating Terms ) the principal portion of the definition for steel is an ironbase alloy, malleable in some temperature range as initially cast, containing manganese, usually carbon, and often other alloying elements. In carbon steel and low-alloy steel, the maximum carbon is about 2.0%; in high-alloy steel, about 2.5%. The dividing line between low-alloy and high-alloy steels is generally regarded as being at about 5% metallic alloying elements (Ref 1). Fundamentally, all steels are mixtures, or more properly, alloys of iron and carbon. However, even the so-called plain-carbon steels have small, but specified, amounts of manganese and silicon plus small and generally unavoidable amounts of phosphorus and sulfur. The carbon content of plain-carbon steels may be as high as 2.0%, but such an alloy is rarely found. Carbon content of commercial steels usually ranges from 0.05 to about 1.0%. The alloying mechanism for iron and carbon is different from the more common and numerous other alloy systems in that the alloying of iron and carbon occurs as a two-step process. In the initial step, iron combines with 6.67% C, forming iron carbide, which is called cementite. Thus, at room temperature, conventional steels consist of a mixture of cementite and ferrite (essentially iron). Each of these is known as a phase (defined as a physically homogeneous and distinct portion of a material system). When a steel is heated above 725 C (1340 F), cementite dissolves in the
2 10 / Practical Heat Treating: Second Edition matrix, and a new phase is formed, which is called austenite. Note that phases of steel should not be confused with structures. There are only three phases involved in any steel ferrite, carbide (cementite), and austenite, whereas there are several structures or mixtures of structures. Classification of Steels It is impossible to determine the precise number of steel compositions and other variations that presently exist, although the total number probably exceeds 1000; thus, any rigid classification is impossible. However, steels are arbitrarily divided into five groups, which has proved generally satisfactory to the metalworking community. These five classes are: Carbon steels Alloy steels (sometimes referred to as low-alloy steels) Stainless steels Tools steels Special-purpose steels The first four of these groups are well defined by designation systems developed by the Society of Automotive Engineers (SAE) and the American Iron and Steel Institute (AISI). Each general class is subdivided into numerous groups, with each grade indentified. The fifth group comprises several hundred different compositions; most of them are proprietary. Many of these special steels are similar to specific steels in the first four groups but vary sufficiently to be marked as separate compositions. For example, the SAE-AISI designation system lists nearly 60 stainless steels in four different general subdivisions. In addition to these steels (generally referred to as standard grades ), there are well over 100 other compositions that are nonstandard. Each steel was developed for a specific application. It should also be noted that both standard and nonstandard steels are designated by the Unified Numbering System (UNS) developed by SAE and ASTM International. Details of this designation system can be found in Ref 2. Coverage in this book, however, is limited to steels of the first four classes carbon, alloy, stainless, and tool steels that are listed by SAE-AISI. Why Steel Is So Important It would be unjust to state that any one metal is more important than another without defining parameters of consideration. For example, without aluminum and titanium alloys, current airplanes and space vechicles could not have been developed.
3 Chapter 2: Fundamentals of the Heat Treating of Steel / 11 Steel, however, is by far the most widely used alloy and for a very good reason. Among layman, the reason for steel s dominance is usually considered to be the abundance of iron ore (iron is the principal ingredient in all steels) and/or the ease by which it can be refined from ore. Neither of these is necessarily correct; iron is by no means the most abundant element, and it is not the easiest metal to produce from ore. Copper, for example, exists as nearly pure metal in certain parts of the world. Steel is such an important material because of its tremendous flexibility in metal working and heat treating to produce a wide variety of mechanical, physical, and chemical properties. Metallurgical Phenomena The broad possibilities provided by the use of steel are attributed mainly to two all-important metallurgical phenomena: iron is an allotropic element; that is, it can exist in more than one crystalline form; and the carbon atom is only 1 30 the size of the iron atom. These phenomena are thus the underlying principles that permit the achievements that are possible through heat treatment. In entering the following discussion of constitution, however, it must be emphasized that a maximum of technical description is unavoidable. This portion of the subject is inherently technical. To avoid that would result in the discussion becoming uninformative and generally useless. The purpose of this chapter is, therefore, to reduce the prominent technical features toward their broadest generalizations and to present those generalizations and underlying principles in a manner that should instruct the reader interested in the metallurgical principles of steel. This is done at the risk of some oversimplification. Constitution of Iron It should first be made clear to the reader that any mention of molten metal is purely academic; this book deals exclusively with the heat treating range that is well below the melting temperature. The objective of this section is to begin with a generalized discussion of the constitution of commercially pure iron, subsequently leading to discussion of the ironcarbon alloy system that is the basis for all steels and their heat treatment. All pure metals, as well as alloys, have individual constitutional or phase diagrams. As a rule, percentages of two principal elements are shown on the horizontal axis of a figure, while temperature variation is shown on the vertical axis. However, the constitutional diagram of a pure metal is a simple vertical line. The constitutional diagram for commercially pure iron is presented in Fig. 1. This specific diagram is a straight
4 12 / Practical Heat Treating: Second Edition line as far as any changes are concerned, although time is indicated on the horizontal. As pure iron, in this case, cools, it changes from one phase to another at constant temperature. No attempt is made, however, to quantify time, but merely to indicate as a matter of interest that as temperature increases, reaction time decreases, which is true in almost any solidsolution reaction. Pure iron solidifies from the liquid at 1538 C (2800 F) (top of Fig. 1). A crystalline structure, known as ferrite, or delta iron, is formed (point a, Fig. 1). This structure, in terms of atom arrangement, is known as a body-centered cubic lattice (bcc), shown in Fig. 2(a). This lattice has nine atoms one at each corner and one in the center. As cooling proceeds further and point b (Fig. 1) is reached (1395 C, or 2540 F), the atoms rearrange into a 14-atom lattice a shown in Fig. 2(b). The lattice now has an atom at each corner and one at the center of each face. This is known as a face-centered cubic lattice (fcc), and this structure is called gamma iron. Fig. 1 Changes in pure iron as it cools from the molten state to room temperature. Source: Ref 3
5 Chapter 2: Fundamentals of the Heat Treating of Steel / 13 As cooling further proceeds to 910 C (1675 F) (point c, Fig. 1), the structure reverts to the nine-atom lattice or alpha iron. The change at point d on Fig. 1 (770 C, or 1420 F) merely denotes a change from nonmagnetic to magnetic iron and does not represent a phase change. The entire field below 910 C (1675 F) is composed of alpha ferrite, which continues on down to room temperature and below. The ferrite forming above the temperature range of austenite is often referred to as delta ferrite; that forming below A 3 as alpha ferrite, though both are structurally similar. In this Greek-letter sequence, austenite is gamma iron, and the interchangeability of these terms should not confuse the fact that only two structurally distinct forms of iron exist. Figures 1 and 2 thus illustrate the allotropy of iron. In the following sections of this chapter, the mechanism of allotropy as the all-important phenomenon relating to the heat treatment of iron-carbon alloys is discussed. Alloying Mechanisms Metal alloys are usually formed by mixing together two or more metals in their molten state. The two most common methods of alloying are by atom exchange and by the interstitial mechanism. The mechanism by which two metals alloy is greatly influenced by the relative atom size. The exchange mechanism simply involves trading of atoms from one lattice system to another. An example of alloying by exchange is the coppernickel system wherein atoms are exchanged back and forth. Fig. 2 Arrangement of atoms in the two crystalline structures of pure iron. (a) Body-centered cubic lattice. (b) Face-centered cubic lattice
6 14 / Practical Heat Treating: Second Edition Interstitial alloying requires that there be a large variation in atom sizes between the elements involved. Because the small carbon atom is 1 30 the size of the iron atom, interstitial alloying is easily facilitated. Under certain conditions, the tiny carbon atoms enter the lattice (the interstices) of the iron crystal (Fig. 2). A description of this basic mechanism follows. Effect of Carbon on the Constitution of Iron As an elemental metal, pure iron has only limited engineering usefulness despite its allotropy. Carbon is the main alloying addition that capitalizes on the allotropic phenomenon and lifts iron from mediocrity into the position of a unique structural material, broadly known as steel. Even in the highly alloyed stainless steels, it is the quite minor constituent carbon that virtually controls the engineering properties. Furthermore, due to the manufacturing processes, carbon in effective quantities persists in all irons and steels unless special methods are used to minimize it. Carbon is almost insoluble in iron, which is in the alpha or ferritic phase (910 C, or 1675 F). However, it is quite soluble in gamma iron. Carbon actually dissolves; that is, the individual atoms of carbon lose themselves in the interstices among the iron atoms. Certain interstices within the fcc structure (austenite) are considerably more accommodating to carbon than are those of ferrite, the other allotrope. This preference exists not only on the mechanical basis of size of opening, however, for it is also a fundamental matter involving electron bonding and the balance of those attractive and repulsive forces that underlie the allotrope phenomenon. The effects of carbon on certain characteristics of pure iron are shown in Fig. 3 (Ref 3). Figure 3(a) is a simplified version of Fig. 1; that is, a straight line constitutional diagram of commercially pure iron. In Fig. 3(b), the diagram is expanded horizontally to depict the initial effects of carbon on the principal thermal points of pure iron. Thus, each vertical dashed line, like the solid line in Fig. 3(a), is a constitutional diagram, but now for iron containing that particular percentage of carbon. Note that carbon lowers the freezing point of iron and that it broadens the temperature range of austenite by raising the temperature A 4 at which (delta) ferrite changes to austenite and by lowering the temperature A 3 at which the austenite reverts to (alpha) ferrite. Hence, carbon is said to be an austenitizing element. The spread of arrows at A 3 covers a two-phase region, which signifies that austenite is retained fully down to the temperatures of the heavy arrow, and only in part down through the zone of the lesser arrows. In a practical approach, however, it should be emphasized that Fig. 1, as well as Fig. 3, represents changes that occur during very slow cooling, as would be possible during laboratory-controlled experiments, rather than under conditions in commercial practice. Furthermore, in slow heating of iron, these transformations take place in a reverse manner. Transforma-
7 Chapter 2: Fundamentals of the Heat Treating of Steel / 15 tions occurring at such slow rates of cooling and heating are known as equilibrium transformations, due to the fact that temperatures indicated in Fig. 1. Therefore, the process by which iron changes from one atomic arrangement to another when heated through 910 C (1675 F) is called a transformation. Transformations of this type occur not only in pure iron but also in many of its alloys; each alloy composition transforms at its own characteristic temperature. It is this transformation that makes possible the variety of properties that can be achieved to a high degree of reproducibility through use of carefully selected heat treatments. Iron-Cementite Phase Diagram When carbon atoms are present, two changes occur (see Fig. 3). First, transformation temperatures are lowered, and second, transformation takes place over a range of temperatures rather than at a single tempera- Fig. 3 Effects of carbon on the characteristics of commercially pure iron. (a) Constitutional diagram for pure iron. (b) Initial effects of carbon on the principal thermal points of pure iron. Source: Ref 3
8 16 / Practical Heat Treating: Second Edition ture. These data are shown in the well-known iron-cementite phase diagram (Fig. 4). However, a word of explanation is offered to clarify the distinction between phases and phase diagrams. A phase is a portion of an alloy, physically, chemically, or crystallographically homogeneous throughout, which is separated from the rest of the alloy by distinct bounding surfaces. Phases that occur in iron-carbon alloys are molten alloy, austenite (gamma phase), ferrite (alpha phase), cementite, and graphite. These phases are also called constituents. Not all constituents (such as pearlite or bainite) are phases these are microstructures. A phase diagram is a graphical representation of the equilibrium temperature and composition limits of phase fields and phase reactions in an alloy system. In the iron-cementite system, temperature is plotted vertically, and composition is plotted horizontally. The iron-cementite diagram (Fig. 4), deals only with the constitution of the iron-iron carbide system, i.e., what phases are present at each temperature and the composition Fig. 4 Iron-cementite phase diagram. Source: Ref 3
9 Chapter 2: Fundamentals of the Heat Treating of Steel / 17 limits of each phase. Any point on the diagram, therefore, represents a definite composition and temperature, each value being found by projecting to the proper reference axis. Although this diagram extends from a temperature of 1870 C (3400 F) down to room temperature, note that part of the diagram lies below 1040 C (1900 F). Steel heat treating practice rarely involves the use of temperatures above 1040 C (1900 F). In metal systems, pressure is usually considered as constant. Frequent reference is made to the iron-cementite diagram (Fig. 4) in this chapter and throughout this book. Consequently, understanding of this concept and diagram is essential to further discussion. The iron-cementite diagram is frequently referred to incorrectly as the iron-carbon equilibrium diagram. Iron- carbon is incorrect because the phase at the extreme right is cementite, rather than carbon or graphite; the term equilibrium is not entirely appropriate because the cementite phase in the iron-graphite system is not really stable. In other words, given sufficient time (less is required at higher temperatures), iron carbide (cementite) decomposes to iron and graphite, i.e., the steel graphitizes. This is a perfectly natural reaction, and only the iron-graphite diagram (see Chapter 12, Heat Treating of Cast Irons ) is properly referred to as a true equilibrium diagram. Solubility of Carbon in Iron In Fig. 4, the area denoted as austenite is actually an area within which iron can retain much dissolved carbon. In fact, most heat treating operations (notably annealing, normalizing, and heating for hardening) begin with heating the alloy into the austenitic range to dissolve the carbide in the iron. At no time during such heating operations are the iron, carbon, or austenite in the molten state. A solid solution of carbon in iron can be visualized as a pyramidal stack of basketballs with golf balls between the spaces in the pile. In this analogy, the basketballs would be the iron atoms, while the golf balls interspersed between would be the smaller carbon atoms. Austenite is the term applied to the solid solution of carbon in gamma iron, and, like other constituents in the diagram, austenite has a certain definite solubility for carbon, which depends on the temperature (shaded area in Fig. 4 bounded by AGFED). As indicated by the austenite area in Fig. 4, the carbon content of austenite can range from 0 to 2%. Under normal conditions, austenite cannot exist at room temperature in plain carbon steels; it can exist only at elevated temperatures bounded by the lines AGFED in Fig. 4. Although austenite does not ordinarily exist at room temperature in carbon steels, the rate at which steels are cooled from the austenitic range has a profound influence on the room temperature
10 18 / Practical Heat Treating: Second Edition microstructure and properties of carbon steels. Thus, the phase known as austenite is fcc iron, capable of containing up to 2% dissolved carbon. The solubility limit for carbon in the bcc structure of iron-carbon alloys is shown by the line ABC in Fig. 4. This area of the diagram is labeled alpha ( ), and the phase is called ferrite. The maximum solubility of carbon in alpha iron (ferrite) is 0.025% and occurs at 725 C (1340 F). At room temperature, ferrite can dissolve only 0.008% C, as shown in Fig. 4. This is the narrow area at the extreme left of Fig. 4 below approximately 910 C (1675 F). For all practical purposes, this area has no effect on heat treatment and shall not be discussed further. Further discussion of Fig. 4 is necessary, although as previously stated, the area of interest for heat treatment extends vertically to only about 1040 C (1900 F) and horizontally to a carbon content of 2%. The large area extending vertically from zero to the line BGH (725 C, or 1340 F) and horizontally to 2% C is denoted as a two-phase area Cm, or alpha (ferrite) plus cementite (carbide). The line BGH is known as the lower transformation temperature (A 1 ). The line AGH is the upper transformation temperature (A 3 ). The triangular area ABG is also a two-phase area, but the phases are alpha and gamma, or ferrite plus austenite. As carbon content increases, the A 3 temperature decreases until the eutectoid is reached 725 C (1340 F) and 0.80% C (point G). This is considered a saturation point; it indicates the amount of carbon that can be dissolved at 725 C (1340 F). A 1 and A 3 intersect and remain as one line to point H as indicated. The area above 725 C (1340 F) and to the right of the austenite region is another two-phase field gamma plus cementite (austenite plus carbide). Now as an example, when a 0.40% carbon steel is heated to 725 C (1340 F), its crystalline structure begins to transform to austenite; transformation is not complete however until a temperature of approximately 815 C (1500 F) is reached. In contrast, as shown in Fig. 4, a steel containing 0.80% C transforms completely to austenite when heated to 725 C (1340 F). Now assume that a steel containing 1.0% C is heated to 725 C (1340 F) or just above. At this temperature, austenite is formed, but because only 0.80% C can be completely dissolved in the austenite, 0.20% C remains as cementite, unless the temperature is increased. However, if the temperature of a 1.0% carbon steel is increased above about 790 C (1450 F), the line GF is intersected, and all of the carbon is thus dissolved. Increasing temperature gradually increases the amount of carbon that can be taken into solid solution. For instance, at 1040 C (1900 F), approximately 1.6% C can be dissolved (Fig.4). Transformation of Austenite Thus far the discussion has been confined to heating of the steel and the phases that result from various combinations of temperature and car-
11 Chapter 2: Fundamentals of the Heat Treating of Steel / 19 bon content. Now what happens when the alloy is cooled? Referring to Fig. 4, assume that a steel containing 0.50% C is heated to 815 C (1500 F). All of the carbon will be dissolved (assuming, of course, that holding time is sufficient). Under these conditions, all of the carbon atoms will dissolve in the interstices of the fcc crystal (Fig. 2b). If the alloy is cooled slowly, transformation to the bcc (Fig. 2a) or alpha phase begins when the temperature drops below approximately 790 C (1450 F). As the temperature continues to decrease, the transformation is essentially complete at 725 C (1340 F). During this transformation, the carbon atoms escape from the lattice because they are essentially insoluble in the alpha crystal (bcc). Thus, in slow cooling, the alloy for all practical purposes, returns to the same state (in terms of phase) that it was before heating to form austenite. The same mechanism occurs with higher carbon steels, except that the austenite-to-ferrite transformation does not go through a two-phase zone (Fig. 4). In addition to the entry and exit of the carbon atoms through the interstices of the iron atoms, other changes occur that affect the practical aspects of heat treating. First, a magnetic change occurs at 770 C (1420 F) as shown in Fig. 1. The heat of transformation effects may chemical changes, such as the heat that is evolved when water freezes into ice and the heat that is absorbed when ice melts. When an iron-carbon alloy is converted to austenite by heat, a large absorption of heat occurs at the transformation temperature. Likewise, when the alloy changes from gamma to alpha (austenite to ferrite), heat evolves. What happens when the alloy is cooled rapidly? When the alloy is cooled suddenly, the carbon atoms cannot make an orderly escape from the iron lattice. This cause atomic bedlam and results in distortion of the lattice, which manifests itself in the form of hardness and/or strength. If cooling is fast enough, a new structure known as martensite is formed, although this new structure (an aggregate of iron and cementite) is in the alpha phase. Classification of Steels by Carbon Content It must be remembered that there are only three phases in steels, but there are many different structures. A precise definition of eutectoid carbon is unavoidable; it varies from 0.77% to slightly over 0.80%, depending on the reference used. However, for the objectives of this book, the precise amount of carbon denoted as eutectoid is of no particular significance. Hypoeutectoid Steels. Carbon steels containing less than 0.80% C are known as hypoeutectoid steels. The area bounded by AGB on the ironcementite diagram (Fig. 4) is of significance to the room temperature microstructures of these steels; within the area, ferrite and austenite each having different carbon contents, can exist simultaneously.
12 20 / Practical Heat Treating: Second Edition Assume that a 0.40% carbon steel has been slowly heated until its temperature throughout the piece is 870 C (1600 F), thereby ensuring a fully austenitic structure. Upon slow cooling, free ferrite begins to form from the austenite when the temperature drops across the line AG, into the area AGB, with increasing amounts of ferrite forming as the temperature continues to decline while in this area. Ideally, under very slow cooling conditions, all of the free ferrite separates from austenite by the time the temperature of the steel reaches A 1 (the line BG) at 725 C (1340 F). The austenite islands, which remain at about 725 C (1340 F), now have the same amount of carbon as the eutectoid steel, or about 0.80%. At or slightly below 725 C (1340 F) the remaining untransformed austenite transforms it becomes pearlite, which is so named because of its resemblance to mother of pearl. Upon further cooling to room temperature, the microstructure remains unchanged, resulting in a final room temperature microstructure of an intimate mixture of free ferrite grains and pearlite islands. A typical microstructure of a 0.40% carbon steel is shown in Fig. 5(a). The pure white areas are the islands of free ferrite grains described previously. Grains that are white but contain dark platelets are typical lamellar pearlite. These platelets are cementite or carbide interspersed through the ferrite, thus conforming to the typical two-phase structure indicated below the BH line in Fig. 4. Eutectoid Steels. A carbon steel containing approximately 0.77% C becomes a solid solution at any temperature in the austenite temperature range, i.e., between 725 and 1370 C (1340 and 2500 F). All of the carbon is dissolved in the austenite. When this solid solution is slowly cooled, several changes occur at 725 C (1340 F). This temperature is a transformation temperature or critical temperature of the iron-cementite system. At this temperature, a 0.77% (0.80%) carbon steels transforms from a single homogeneous solid solution into two distinct new solid phases. This change occurs at constant temperature and with the evolution of heat. The new phases are ferrite an cementite, formed simultaneously; however, it is only at composition point G in Fig. 4 (0.77% carbon steel) that this phenomenon of the simultaneous formation of ferrite and cementite can occur. The microstructure of a typical eutectoid steel is shown in Fig. 5(b). The white matrix is alpha ferrite and the dark platelets are cementite. All grains are pearlite no free ferrite grains are present under these conditions. Cooling conditions (rate and temperature) govern the final condition of the particles of cementite that precipitate from the austenite at 725 C (1340 F). Under specific cooling conditions, the particles become spheroidal instead of elongated platelets as shown in Fig. 5(b). Figure 5(c) shows a similar two-phase structure resulting from slowly cooling a eutectoid carbon steel just below A 1. This structure is commonly known as
13 Chapter 2: Fundamentals of the Heat Treating of Steel / 21 spheroidite but is still a despersion of cementite particles in alpha ferrite. There is no indication of grain boundaries in Fig. 5(c). The spheroidized structure is often preferred over the pearlitic structure because spheroidite has superior machinability and formability. Combination structures (that is, partly lamellar and partly spheroidal cementite in a ferrite matrix) are also common. As noted previously, a eutectoid steel theoretically contains a precise amount of carbon. In practice, steels that contain carbon within the range of approximately 0.75 to 0.85% are commonly referred to as eutectoid carbon steels. Hypereutectoid steels contain carbon contents of approximately 0.80 to 2.0%. Assume that a steel containing 1.0% C has been heated to 845 C (1550 F), thereby ensuring a 100% austenitic structure. When cooled, no Fig. 5 Effects of carbon content on the microstructures of plain-carbon steels. (a) Ferrite grains (white) and pearlite (gray streaks) in a white matrix of a hypoeutectoid steel containing 0.4% C (b) Microstructure (all pearlite grains) of a eutectoid steel containing 0.77% C (c) Microstructure of a eutectoid steel containing 0.77% C with all cementite in the spheroidal form (d) Microstructure of a hypereutectoid steel containing 1.0% C containing pearlite with excess cementite bounding the grains Source: Ref 4
14 22 / Practical Heat Treating: Second Edition change occurs until the line GF (Fig. 4), known as A cm or cementite solubility line, is reached. At this point, cementite begins to separate out from the austenite, and increasing amounts of cementite separate out as the temperature of the 1% carbon steels descends below the A line. The composition of austenite changes from 1% C toward 0.77% C. At a temperature slightly below 725 C (1340 F), the remaining austenite changes to pearline. No further changes occur as cooling proceeds toward room temperature, so that the room temperature microstructure consists of pearline and free cementite. In this case, the free cementite exists as a network around the pearline grains (Fig. 5d). Upon heating hypereutectoid steels, reverse changes occur. At 725 C (1340 F), pearlite changes to austenite. As the temperature increases above 725 C (1340 F), free cementite dissolves in the austenite, so that when the temperature reaches the A cm line, all the cementite dissolves to form 100% austenite. Hysteresis in Heating and Cooling The critical temperatures (A 1,A 6, and A cm ) are arrests in heating or cooling and have been symbolized with the letter A, from the French word arret meaning arrest or a delay point, in curves plotted to show heating or cooling of samples. Such changes occur at transformation temperatures in the iron-cementite diagram if sufficient time is given and cab be plotted for steels showing lags at transformation temperatures, as shown for iron in Fig. 4. However, because heating rates in commercial practice usually exceed those in controlled laboratory experiments, changes on heating usually occur at temperatures a few degrees above the transformation temperatures shown in Fig. 4 and are known as Ac temperatures, such as Ac 1 or Ac 3. The c is from the French word chauffage, meaning heating. Thus, Ac 1 is a few degrees above the ideal A 1 temperature. Likewise, on slow cooling in commercial practice, transformation changes occur at temperatures a few degrees below those in Fig. 4. These are known as Ar, or Ar 3, the r originating from the French word refroidissement, meaning cooling. This difference between the heating and cooling varies with the rate of heating or cooling. The faster the heating, the higher the Ac point; the faster the cooling, the lower the Ar point. Also, the faster the heating and cooling rate, the greater the gap between the Ac and Ar points of the reversible (equilibrium) point A. Going one step further, in cooling a piece of steel, it is of utmost importance to note that the cooling rate may be so rapid (as in quenching steel in water) as to suppress the transformation for several hundreds of degrees. This is due to the decrease in reaction rate with decrease in temperature. As discussed subsequently, time is an important factor in transformation, especially in cooling.
15 Chapter 2: Fundamentals of the Heat Treating of Steel / 23 Effect of Time on Transformation The foregoing discussion has been confined principally to phases that are formed by various combinations of composition and temperature; little reference has been made to the effects of time. In order to convey to the reader the effects of time on transformation, the simplest approach is by means of a time-temperature-transformation (TTT) curve for some constant iron-carbon composition. Such a curve is presented in Fig. 6 for a 0.77% (eutectoid) carbon steel. TTT curves are also known as S curves because the principal part of the curve is shaped like the letter S. In Fig. 6, temperature is plotted on the vertical axis, and time is plotted on a logarithmic scale along the horizontal axis. The reason for plotting time on a logarithmic scale is merely to keep the width of the chart within a manageable dimension. In analyzing Fig. 6, begin with line Ae 1 (725 C or 1340 F). Above this temperature, austenite exists only for a eutectoid steel (refer also to Fig. 4). When the steel is cooled and held at a temperature just below Ae 1 (705 C or 1300 F), transformation begins (follow line (P s B s ), but very slowly at this temperature;1 h of cooling is required before any significant amount of transformation occurs, although eventually complete transformation occurs isothermally (meaning at a constant temperature), and the transformation product is spheroidite (Fig. 5c). Now assume a lower temperature (650 C or 1200 F) on line P s B s (the line of beginning transformation); transformation begins in less than 1 min, and the transfor- Fig. 6 Time-temperature-transformation (TTT) diagram for a eutectoid (0.77%) carbon steel. Source: Ref 3
16 24 / Practical Heat Treating: Second Edition mation product is coarse pearlite (near the right side of Fig. 6). Next, assume a temperature of 540 C (1000 F); transformation begins in approximately 1 s and is completely transformed to fine pearlite in a matter of a few minutes. The line P f B f represents the completion of transformation and is generally parallel with P s B s. However, if the steel is cooled very rapidly (such as by immersing in water) so that there is not sufficient time for transformation to begin in the 540 C (1000 F) temperature vicinity, then the beginning of transformation time is substantially extended. For example, if the steel is cooled to and held at 315 C (600 F), transformation does not begin for well over 1 min. It must be remembered that all of the white area to the left of line P s B s represents the austentic phase, although it is highly unstable. When transformation takes place isothermally within the temperature range of approximately 290 to 425 C (550 to 800 F), the transformation product is a microstructure called bainite (upper or lower as indicated toward the right of Fig. 6). A bainitic microstructure is shown in Fig. 7(b). In another example, steel is cooled so rapidly that no transformation takes place in the 540 C (1000 F) region and rapid cooling is continued (note line XY in Fig. 6) to and below 275 C (530 F) or M s. Under these conditions, martensite is formed. Point M s is the temperature at which martensite begins to form, and M f indicates the complete finish of transformation. It must be remembered that martensite is not a phase but is a specific microstructure in the ferritic (alpha) phase. Martensite is formed from the carbon atoms jamming the lattice of the austenitic atomic arrangement. Thus, martensite can be considered as an aggregate of iron and cementite (Fig. 7a). In Fig. 6, the microstructure of austenite (as it apparently appears at elevated temperature) is shown on the right. It is also evident that the lower the temperature at which transformation takes place, the higher the hardness (see Chapter 3, Hardness and Hardenability ). Fig. 7 (a) Microstructure of quenched 0.95% carbon steel Structure is martensitic. (b) Bainitic structure in a quenched 0.95% carbon steel Source: Ref 4
17 Chapter 2: Fundamentals of the Heat Treating of Steel / 25 It is also evident that all structures from the top to the region where martensite forms (Ae 1 ) are time-dependant, but the formation of martensite is not time-dependent. Each different steel composition has its own TTT curve; Fig. 6 is presented only as an example. However, patterns are much the same for all steels as far as shape of the curves is concerned. The most outstanding difference in the curves among different steels is the distance between the vertical axis and the nose of the S curve. This occurs at about 540 C (1000 F) for the steel in Fig. 6. This distance in terms of time is about 1 s for a eutectoid carbon steel, but could be an hour or more for certain high-alloy steels, which are extremely sluggish in transformation. The distance between the vertical axis and the nose of the S curve is often called the gap and has a profound effect on how rapidly the steel must be cooled to form the hardened structure martensite. Width of this gap for any steel is directly related to the critical cooling rate for that specific steel. Critical cooling rate is defined as the rate at which a given steel must be cooled from the austenite to prevent the formation of nonmartensitic products. In Fig. 6, it is irrelevant whether the cooling rate follows the lines X to Y or X to Z because they are both at the left of the beginning transformation line P s B s. Practical heat treating procedures are based on the fact that once the steel has been cooled below approximately 425 C (800 F), the rate of cooling may be decreased. These conditions are all closely related to hardenability, which is dealt with in Chapter 3. REFERENCES 1. H.E. Boyer, Chapter 1, Practical Heat Treating, 1st ed., American Society for Metals, 1984, p Metals & Alloys in the Unified Numbering System, 10th ed, SAE International and ASTM International, H.N. Oppenheimer, Heat Treatment of Carbon Steels, Course 42, Lesson 1, Practical Heat Treating, Materials Engineering Institute, ASM International, H.E. Boyer, Chapter 2, Practical Heat Treating, 1st ed., American Society for Metals, 1984, p SELECTED REFERENCES C.R. Brooks, Principles of the Heat Treatment of Plain Carbon and Low Alloy Steels, ASM International, 1996 Atlas of Time-Temperature Diagrams for Irons and Steels, G.F. Vander Voort, Ed., ASM International, 1991 G. Krauss, Steels: Processing, Structure, and Performance, ASM International, 2005
Iron-Carbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
Section 3: HEAT TREATMENT Introduction Objectives of Heat Treatment Heat Treatment is the controlled heating and cooling of metals to alter their physical and mechanical properties without changing the
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
9-2 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
High-Strength Low-Alloy Steels Introduction and Overview High-strength low-alloy (HSLA) steels, or microalloyed steels, are designed to provide better mechanical properties and/or greater resistance to
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
INDUSTRIAL MATERIALS Development of High-Strength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai High-carbon
Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi-221
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low
How annealing, stress relief and aging each affect the mechanical properties of spring materials By Terry Bartel Elgiloy Specialty Metals In the metals industry, there are numerous steps from the raw material
Problem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength - high conductivity electrical leads to integrated circuits
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
Structure of Metals 110 Welcome to the Tooling University. This course is designed to be used in conjunction with the online version of this class. The online version can be found at http://www.toolingu.com.
ecture 18-22: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
METALLURGY OVERVIEW FERROUS AND NON-FERROUS Metalworking fluids are exactly what the term means: the fluids are used to work the metal. The work can be any method that changes the shape of the metal. This
Designation: A 56 84 (Reapproved 999) e Standard Specification for Ductile Iron Castings This standard is issued under the fixed designation A 56; the number immediately following the designation indicates
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
Lecture 1: Kinetics vs. Thermodynamics: different but related Today s topics The basic concepts of Kinetics and Thermodynamics, and how to understand the difference and inter-relationship between the two
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view
Study on the Mechanism of Strengthening and Toughening Effect of Titanium Addition on HSLA Steel FANG Jian Abstract: Based on the determination of load variation against deflection by means of Instrumented
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, firstname.lastname@example.org;
Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what
TM A high hardness, corrosion and fatigue resistance martensitic grade CONTINUOUS METALLURGICAL SPECIAL STEELS INNOVATION RESEARCH SERVICE DEVELOPMENT Enhancing your performance THE INDUSTRIAL ENVIRONMENT
MSE 528 - PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of Al-Zn-Mg-Cu high strength alloy on isothermal
INDUCTION WELDED SMALL DIAMETER TUBE PRODUCTION LINE Target Production of welded single - wall tubing manufactured to ASTM A 513, also zinc coated as per UNI 5741-66, suitable for many low pressure and
8. Technical Heat Treatment 8. Technical Heat Treatment 95 6 cm 4 2 0-2 -4 C 400 C C -6-14 -12-10 -8-6 -4-2 0 2 cm 6 723 C temperature C 1750 750 250 When welding a workpiece, not only the weld itself,
Engineering Material Ferrous material; A general classification of engineering materials is shown in Figure 1.8. Engineering material can be broadly classified as Metallic and Non-Metallic materials. The
FATIGUE BEHAVIOUR ANALYSIS OF DIFFERENTLY HEAT TREATED MEDIUM CARBON STEEL A THESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENTS FOR THE DEGREE OF Master of Technology (Res.) in Metallurgical and
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
Introduction: North American Stainless Flat Products Stainless Steel Grade Sheet 309S (S30908)/ EN1.4833 SS309 is a highly alloyed austenitic stainless steel used for its excellent oxidation resistance,
WELDING AND COATING METALLURGY 1 INTRODUCTION 4 1.1 ROLE OF CARBON IN STEEL 4 1.2 WELDABILITY OF STEELS 5 2 CRYSTAL STRUCTURE 7 2.1 SOLUBILITY OF CARBON 8 3 IRON - IRON CARBIDE PHASE DIAGRAM 9 3.1 AUSTENITE
North American Stainless Flat Products Stainless Steel Grade Sheet 430 (S43000)/ EN 1.4016 Introduction: SS430 is a low-carbon plain chromium, ferritic stainless steel without any stabilization of carbon
North American Stainless Flat Products Stainless Steel Grade Sheet 310S (S31008)/ EN 1.4845 Introduction: SS310 is a highly alloyed austenitic stainless steel designed for elevated-temperature service.
ATI 316Ti Stainless Steel: Austenitic (UNS S31635) GENERAL PROPERTIES ATI 316Ti stainless is a titanium-stabilized version of Type 316 molybdenum-bearing austenitic stainless steel. It is also known as
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
304/304L STAINLESS STEEL P r o d u c t D ata B u l l e t i n Architectural Moldings and Trim Textile Kitchen Equipment Paper Pharmaceutical and Chemical Industry Processing Equipment High strength, excellent
North American Stainless Long Products Stainless Steel Grade Sheet AISI 310S S31008 EN 1.4845 AISI 314 S31400 EN 1.4841 INTRODUCTION Types 310S SS and 314 SS are highly alloyed austenitic stainless steels
Lecture Notes: Mixtures, Compounds & Solutions The physical properties of any substance include size, shape, state, and color. Changing a physical property of a substance does not change the chemical make-up.
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
Ionic and Metallic Bonding BNDING AND INTERACTINS 71 Ions For students using the Foundation edition, assign problems 1, 3 5, 7 12, 14, 15, 18 20 Essential Understanding Ions form when atoms gain or lose
Heat Treatment of Iron 2009 by David A. Katz. All rights reserved, Department of Chemistry Pima Community College The purpose of this experiment is to investigate the effects of heat-treating on the properties
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of X-ray diffraction techniques for investigating various types
EVALUATION METHODS OF DILATOMETER CURVES OF PHASE TRANSFORMATIONS Petr MOTYČKA 1, Michal KÖVÉR 1,2 1 COMTES FHT a.s., Průmyslová 995, Dobřany, Czech Republic, 2 Slovak University of Technology in Bratislava,
A Stainless Steel Primer Part 1: The Types of Stainless Steel By John C. Tverberg [This is the first of a three part series of articles on the use of stainless steel and nickel alloys in the fluid control
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module - 2 Lecture - 2 Part 2 of 2 Review of Atomic Bonding II We will continue
Journal of Minerals & Materials Characterization & Engineering, Vol. 10, No.3, pp.299-308, 2011 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment on Mechanical Properties and Microstructure
s 410, 420, 425 Mod, and 440A GENERAL PROPERTIES s 410, 420, 425 Modified, and 440A (see composition on Page 2) are hardenable, straight-chromium stainless steels which combine superior wear resistance
Describe the strength of attractive forces between particles. Describe the amount of space between particles. Can the particles in this state be compressed? Do the particles in this state have a definite
Associate Professor Su-Jin Kim School of Mechanical Engineering Gyeongsang National University Outline 1. Physics 2. Sand 3. Investment 4. Die 5. Cost/Quality is a manufacturing process by which a liquid
Heat Treating Aluminum Alloys Any sufficiently advanced technology is indistinguishable from magic Arthur C Clarke Disclaimer This information is provided as-is/where-is with no warranty expressed or implied.
9-13 9.8: 9.11 Upon heating a lead-tin alloy of composition 30 wt% Sn-70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
Module 3 Machinability Lesson 1 Cutting Tool Materials of common use Instructional Objectives At the end of this lesson, the students will be able to (i) Identify the needs and cite the chronological development
Data Sheet: A2.2 High carbon and quenchable steels Hot Rolled Steel Plate and Coil for Hardening and Wear Resistance General description Steel is generally classified as high carbon steel if the nominal
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
CLASS PROGRAMME Approval of manufacturers DNVGL-CP-0249 Edition May 2016 The content of this service document is the subject of intellectual property rights reserved by ("DNV GL"). The user accepts that
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H-1111 Budapest, Goldmann tér 3. Summary In this
ME 212 LABORATORY EXPERIMENT #3 HARDNESS TESTING AND AGE HARDENING 1. OBJECTIVE Our primary aim is to measure the Rockwell Hardness values of materials and estimate ultimate tensile strengths by the aid
Technical Data BLUE SHEET Allegheny Ludlum Corporation Pittsburgh, PA Martensitic Stainless Steels Types 410, 420, 425 Mod, and 440A GENERAL PROPERTIES Allegheny Ludlum Types 410, 420, 425 Modified, and
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.35-153.881-412.2=20 RAPIDLY SOLIDIFIED COPPER ALLOYS RIBBONS M. ŠULER 1, L. KOSEC 1, A. C. KNEISSL 2, M. BIZJAK 1, K. RAIĆ
Tables of contents 1. Discuss the properties of plain carbon steel.... 2 About steel... 2 Plain carbon steel... 2 General properties of plain carbon steel... 2 Physical properties of plain carbon steel....
North American Stainless Long Products Stainless Steel Grade Sheet 2205 UNS S2205 EN 1.4462 2304 UNS S2304 EN 1.4362 INTRODUCTION Types 2205 and 2304 are duplex stainless steel grades with a microstructure,
EXAMPLE EXERCISE 4.1 Change of Physical State State the term that applies to each of the following changes of physical state: (a) Snow changes from a solid to a liquid. (b) Gasoline changes from a liquid
Your consent to our cookies if you continue to use this website.